2 Imperfections in Solids The properties of some materials are profoundly influenced by the presence of imperfections.It is important to have knowledge about the types of imperfections that exist and the roles they play in affecting the behavior of materials.
3 Atom Purity and Crystal Perfection If we assume a perfect crystal structure containing pure elements, then anything that deviated from this concept or intruded in this uniform homogeneity would be an imperfection.There are no perfect crystals.Many material properties are improved by the presence of imperfections and deliberately modified (alloying and doping).
5 Point Defects in Metals • Vacancies:-vacant atomic sites in a structure.Vacancydistortionof planes• Self-Interstitials:-"extra" atoms positioned between atomic sites.self-interstitialdistortionof planes
6 Self Interstitialsc05f01In metals, a self interstitial introduces relatively large distortions (strain) in the surrounding lattice since the atom is substantially larger than the interstitial site.
7 Point Defects in Ceramics • Vacancies-- vacancies exist in ceramics for both cations and anions• Interstitials-- interstitials exist for cations-- interstitials are not normally observed for anions because anions are large relative to the interstitial sitesCation InterstitialCation VacancyAnion VacancyAdapted from Fig. 5.2, Callister & Rethwisch 3e. (Fig. 5.2 is from W.G. Moffatt, G.W. Pearsall, and J. Wulff, The Structure and Properties of Materials, Vol. 1, Structure, John Wiley and Sons, Inc., p. 78.)
8 Point Defects: Frenkel and Schottky • Frenkel DefectTo maintain the charge neutrality, a cation vacancy-cation interstitial pair occur together. The cation leaves its normal position and moves to the interstitial site.• Schottky DefectTo maintain the charge neutrality, remove 1 cation and 1 anion;this creates 2 vacancies.SchottkyDefectFrenkelAdapted from Fig. 5.3, Callister & Rethwisch 3e. (Fig. 5.3 is from W.G. Moffatt, G.W. Pearsall, and J. Wulff, The Structure and Properties of Materials, Vol. 1, Structure, John Wiley and Sons, Inc., p. 78.)
9 Equilibrium Concentration: Point Defects • Equilibrium concentration varies with temperature.Activation energy –energy required for formation of vacancyNo. of defectsæöNQvçv÷=expç÷No. of potentialèøNkTdefect sitesTemperatureBoltzmann's constant-23(1.38 x 10J/atom-K)-5(8.62x10eV/atom-K)Each lattice siteis a potentialvacancy site
10 Measuring Activation Energy ç÷Nv=exp-QkTæèöø• We can get Qv froman experiment.• Measure this...NvTexponentialdependence!defect concentration• Replot it...1/TNvln-Q/kslope
11 Estimating Vacancy Concentration • Find the equil. # of vacancies in 1 m3 of Cu at 1000C.• Ex Given:r= 8.4 g/cm3A= 63.5 g/molCuQ= 0.9 eV/atomN= 6.02 x 1023atoms/molvA8.62 x 10-5eV/atom-K0.9 eV/atom1273 Kç÷Nv=exp-QkTæèöø= 2.7 x 10-4For 1 m3, N =NACurx1 m3= 8.0 x 1028 sites• Answer:Nv=(2.7 x 10-4)(8.0 x 1028) sites = 2.2 x 1025 vacancies
12 Point Defects in Polymers Defects due in part to chain packing errors and impurities such as chain ends and side chainsAdapted from Fig. 5.7, Callister & Rethwisch 3e.
13 AlloyingGiven a metal (with only 1 type of atom) refined to % purity, there would still exist 1022 to 1023 impurity atoms in 1 cubic meter of material.Most metals are alloys. Alloying is done to improve strength, corrosion resistance, ductility, lower melting T.For example, sterling silver is an alloy of 92.5% silver, 7.5% copper. At room temperature, “pure” silver is highly corrosion resistant, but also very soft. The addition of copper improves the strength and maintains good corrosion behavior.
14 Solid SolutionThe addition of impurity atoms to a metal results in the formation of a solid solution.The solvent represents the element that is present in the greatest amount (the host atoms). For example, in Lab 8 (MSE 227) Precipitation Hardening of Aluminum, aluminum is the solvent and copper is the solute (present in minor concentration ).Solid solutions form when the solute atoms (Cu) are added to the solvent (Al), assuming the crystal structure is maintained and no new structures are formed.
15 Solid Solution - continued A solid solution is a homogenous composition throughout.The impurity atoms (Cu) are randomly and uniformly dispersed within the solid.The impurity defects in the solid solution are either substitutional or interstitial.
16 Imperfections in Metals What are the outcomes if impurity (B) is added to host (A)?• Solid solution of B in A (random distribution of point defects)ORSubstitutional solid solution.(e.g., Cu in Ni)Interstitial solid solution.(e.g., C in Fe)• Solid solution of B in A plus particles of a newphase (usually for a larger amount of B)Second phase particle-- different composition-- often different structure.
17 Hume - Rothery RulesThe Hume-Rothery rules are basic conditions for an element to dissolve in a metal, forming a substitutional solid solution.The atomic radius of the solute and solvent atoms must differ by no more than 15% (r < 15%).The solute and solvent should have similar electronegativities.Same crystal structure for “pure” metals.Maximum solubility occurs when the solvent and solute have the same valence. Metals with lower valence will tend to dissolve metals with higher valence.
18 Substitutional Solid Solution Example: Copper and Nickel Element Atomic Crystal Electro- Valence Radius Structure nega- (nm) tivityCu FCC C H O Ag FCC Al FCC Co HCP Cr BCC Fe BCC Ni FCC Pd FCC Zn HCP
19 Interstitial Solid Solution Carbon forms an interstitial solid solution when added to iron; the maximum concentration of carbon that can be added is roughly 2%.The atomic radius of the carbon atom is much less than that of iron (0.071nm vs nm).For interstitial solid solutions, the Hume-Rothery rules are:1. Solute atoms must be smaller than the pores in the solvent lattice.2. The solute and solvent should have similar electronegativity.
20 Imperfections in Ceramics • Since there are both anions and cations in ceramics, a substitutional impurity will replace the host ion most similar in terms of charge.Charge balance must be maintained when impurities are present.• Ex: NaClNa+Cl-• Substitutional cation impuritywithout impurityCa2+impuritywith impurityNa+cationvacancy• Substitutional anion impuritywithout impurityO2-impurityCl-anion vacancywith impurity
23 Line Defects Dislocations: Schematic of Zinc (HCP): slip steps • are line defects,• slip between crystal planes result when dislocations move,• produce permanent (plastic) deformation.Schematic of Zinc (HCP):• before deformation• after tensile elongationslip steps
24 Imperfections in Solids Linear defects (Dislocations) are one-dimensional defects that cause misalignment of nearby atoms.Linear defects are associated primarily with mechanical deformation.Types of dislocations: edge, screw, mixed.Edge dislocation:extra half-plane of atoms inserted in a crystal structure; the edge of the plane terminates within the crystal.Around the dislocation line there is some localized distortion.b perpendicular () to dislocation lineBurger’s vector, b: measure of lattice distortion2424
25 Motion of Edge Dislocation • Dislocation motion requires the successive bumpingof a half plane of atoms (from left to right).• Bonds across the slipping planes are broken andremade in succession.The (plastic) permanent deformation of most crystalline materials is by dislocation movement.Most contain some dislocations that were introduced during solidification, plastic deformations, and rapid cooling (thermal stresses).To deform plastically means to slide atomic planes past each other.Atomic view of edgedislocation motion fromleft to right as a crystalis sheared.
26 DislocationsThe strength of a material with no dislocations is times greater than the strength of a material with a high dislocation density.So, materials with no dislocations may be very strong, but they cannot be deformed.The dislocations weaken a material, but make plastic deformation possible.
27 Imperfections in Solids Screw dislocation:Named for the spiral stacking of crystal planes around the dislocation line; results from shear deformationb parallel () to dislocation line
29 Characteristics of Dislocations During plastic deformation, the number of dislocations increase dramatically to densities of 1010 mm-2.Grain boundaries, internal defects and surface irregularities serve as formation sites for dislocations during deformation.
30 Dislocations During Cold Working Ti alloy after cold working.Dislocations entangle with one another during cold work.Dislocation movement becomes more difficult.Dislocations are visible in electron micrographs
33 Polycrystalline Materials Grain Boundariesregions between crystalstransition from lattice of one region to anotherThe atoms near the boundaries of the 3 grains do not have an equilibrium spacing or arrangement; slightly disordered.Grains and grain boundaries in a stainless steel sample. low density in grain boundaries
34 Planar Defects in Solids - Twinning A shear force that causes atomic displacements such that the atoms on one side of a plane (twin boundary) mirror the atoms on the other side. A reflection of atom positions across the twin plane.Displacement magnitude in the twin region is proportional to the atom’s distance from the twin plane.Takes place along defined planes and directions depending upon the system.Ex: BCC twinning occurs on the (112) system
35 Twinning Stacking faults (c) 2003 Brooks/Cole Publishing / Thomson LearningApplied stress to a perfect crystal (a) may cause a displacement of the atoms, (b) causing the formation of a twin. Note that the crystal has deformed as a result of twinning.Stacking faultsFor FCC metals an error in ABCABC packing sequenceEx: ABCABABC
36 Properties of Twinning Of the three common crystal structures BCC, FCC and HCP, the HCP structure is the most likely to twin.FCC structures will not usually twin because slip is more energetically favorable.Twinning occurs at low temperatures and high rates of shear loading (shock loading) conditions where there are few present slip systems (restricting the possibility of slip)Small amount of deformation when compared with slip.
38 Slip SystemsUsually there are preferred slip planes and directions in crystal systems.The combination of both the slip plane and direction form the slip system.Slip plane is generally taken as the closest packed plane in the systemSlip direction is taken as the direction on the slip plane with the highest linear density.
39 Slip systemsFCC and BCC materials have large numbers of slip systems (at least 12) and are considered ductile.HCP systems have few slip systems and are quite brittle.
43 Microscopic Examination Metallography – sample preparation is necessary to examine the surface of materials (metals, ceramics, polymers).A smooth mirror-like finish is obtained by grinding and polishing using successively finer abrasive papers and powder mixed with water.The microstructure (grain size, shape, orientation) is revealed using a chemical reagent (etching solution) on a polycrystalline sample.Etching characteristics vary from grain to grain.
44 Optical Microscopy • Useful up to 2000X magnification. • Polishing removes surface features (e.g., scratches)• Etching changes reflectance, depending on crystalorientation.0.75mmcrystallographic planesMicrograph ofbrass (a Cu-Zn alloy)
45 Optical Microscopy Grain boundaries... Fe-Cr alloy N = 2 n -1 grain boundarysurface groovepolished surface(a)• are imperfections,• are more susceptibleto etching,• may be revealed asdark lines,• change in crystalorientation acrossboundary.ASTM grainsize numberN= 2n-1number of grains/in2at 100xmagnificationAdapted from Fig. 5.19(a) and (b), Callister & Rethwisch 3e. (Fig. 5.19(b) is courtesyof L.C. Smith and C. Brady, the National Bureau of Standards, Washington, DC [now the National Institute of Standards and Technology, Gaithersburg, MD].)
48 Microscopy Optical (light) resolution (0.1 m = 100 nm = 10-7 m) For higher resolution need higher frequencyX-Rays are difficult to focus.Electronswavelengths are roughly 3 pm (0.003 nm)(Magnification - 1,000,000X)Atomic resolution possibleElectron beam focused by magnetic lenses.
Your consent to our cookies if you continue to use this website.